O R I G I N A L A R T I C L E
Effects of water soaking and outdoor exposure on modulus
of rupture and internal bond strength of particleboard
Hideaki Korai•Hiroshi Saotome• Masaharu Ohmi
Received: 9 May 2013 / Accepted: 2 October 2013 / Published online: 29 November 2013 ÓThe Japan Wood Research Society 2013
Abstract Phenol–formaldehyde resin-bonded board (PF board) and isocyanate resin-bonded particle-board (MDI particle-board) were soaked in water at 40, 70 and 100°C, and the relationships between soaking conditions and board properties were analyzed. The relationships between the deterioration of board properties resulting from water soaking and those arising from outdoor expo-sure were also analyzed. At 100°C, the modulus of rupture (MOR) and internal bond strength (IB) of the PF board decreased significantly within the first hour, and subse-quently constant values were shown with increasing soaking time. This low constant value was defined as the lower limit. At 70°C, both the MOR and IB decreased with increasing soaking time, and reached the lower limit. At 40°C, however, neither decreased significantly with increasing soaking time and neither reached the lower limit. The MOR of the MDI board showed the same trend as the PF board. However, the IB of the MDI board showed a different trend to the PF board, that is, the lower limit of IB required extensive soaking, even at 100°C. The MOR and IB of both the PF and MDI boards reached the lower limit when thickness change peaked. On the other hand, the MOR and IB for outdoor exposure were lower than those for water soaking, even at the same thickness change. The
MOR and IB of water soaking decreased owing to the collapse of the bonding points caused by board swelling. On the other hand, the board properties of outdoor expo-sure decreased owing to the collapse of the bonding points, and biodegradation also added to the decrease.
Keywords ParticleboardWater soakingOutdoor exposureAccelerated aging Bonding point
In order to evaluate the durability of wood-based boards, various accelerated aging tests are used [1–3]. Most involve water soaking at various temperatures. In JIS A 5908, for example, the A test is 2 h water soaking at 70°C, and the B test is 2 h water soaking at 100°C . For the Engineered Wood Products Association, the test is 8 h water soaking at 66 °C followed by 14.5 h drying at 82°C . Although the most widely used accelerated aging test is water soaking at various temperatures and times, no optimum test has yet been decided upon.
Numerous studies have been made on the relationships between cyclic boil-dry treatment and board properties [6– 8], but very few have detailed the effects of water-soaking condition on board properties. For example, when we compare 2 h water soaking at 70°C (A test in JIS) and 2 h water soaking at 100°C (B test in JIS), obviously the latter is more severe than the former, decreasing the latter properties more than the former . Comparing 6 h water soaking at 70°C with 2 h water soaking at 100°C, it is very difficult to predict which condition decreases the board properties. In order to develop an optimum accel-erated aging test, it is paramount to determine the effects of soaking temperature and time on board properties. Part of this article was presented at the 30th (Tokyo, October 2012)
annual meeting of the Wood Technology Association of Japan.
H. Korai (&)H. Saotome
Forestry and Forest Products Research Institute, Tsukuba 305-8687, Japan
Faculty of Agriculture, Tokyo University of Agriculture and Technology, Tokyo 183-8509, Japan
Thereby, the purpose of this study is to clarify the roles played by soaking temperature and time.
The reason for decrease in board properties is the col-lapse of the bonding points of the binder [9,10]. This col-lapse results from wood failure (Fig.1b), decomposition of the binder (cohesive failure, Fig.1c) and the reduction of bonding strength between the binders and the element sur-face (particle sursur-face in this study; intersur-face failure, Fig.1d) . When boards are manufactured, the particles are compressed into a high-density structure. As a result, swelling stress is generated within the particles owing to spring-back, and this swelling stress is released when the particles swell owing to water soaking. Phenol–formalde-hyde resin and isocyanate resin are highly durable to water , and do not decompose when soaked in water, even at 100°C; thus, both cohesive failure and wood failure hardly occur after swelling stress is released. Accordingly, the bonding points must inevitably collapse as a result of interface failure. When a board swells to maximum thick-ness, the board properties presumably cease to fail. After a certain increase in the soaking time, the values remained constant; and this low constant value is defined as the lower limit in this study, and we also confirm this matter.
As for failure resulting from outdoor exposure, boards were exposed outdoors at eight sites in Japan for 7 years (2004–2011), and their properties were evaluated [13–15]. The relationships between the reduction of board properties owing to water soaking and those owing to outdoor exposure were then compared and analyzed.
Particleboards used in this experiment
Phenol–formaldehyde resin-bonded particleboard (PF board) and isocyanate resin-bonded particleboard (MDI board) were used in the experiments. The density and thickness of the boards were 0.75 g/cm3and 12.2 mm for the PF board and 0.80 g/cm3 and 12.1 mm for the MDI board, respectively. Further details are provided in the
references [10,13–15]. The boards were commercial pro-ducts that did not include detailed information such as binder content. Both types of boards satisfied the water-proof category of Type 18 and Type P under JIS A 5908 . Type 18 satisfies 18 MPa in modulus of rupture (MOR) and Type P indicates waterproof boards. The initial MOR and internal bond strength (IB) of the PF board were 20.3 (2.29) and 0.83 (0.09) MPa, respectively. The number in parentheses indicates the standard deviation. The initial MOR and IB of the MDI board were 28.8 (2.10) and 2.19 (0.18) MPa, respectively. The MOR and IB tests were conducted in compliance with JIS . The number of specimens for measuring the initial values of MOR and IB each was 30.
For the MOR tests, board specimens measuring 275 950 mm were soaked in water at 40, 70, and 100 °C. Soaking times at 40 °C were 2, 12, and 336 h; at 70°C 1, 2, 6, 24, and 168 h; and at 100°C 1, 2, 6, 24, and 72 h. The number of specimens for the MOR tests was five. The specimens were dried in an oven at 30°C for 48 h, and subsequently, were conditioned at a constant temperature of 20 °C and relative humidity of 65 % for 7–10 days until the weight stabilized. The moisture content of the speci-mens was approximately 10 %. After conditioning, the thickness of the specimens was first measured in order to determine thickness changes (TC), and then, the MOR tests were conducted. After the MOR tests, specimens measur-ing 50950 mm were taken from the two edges of the original 275 950 mm specimens for the IB tests, and subsequent IB tests were conducted. The number of MOR and IB tests was five and ten, respectively. The MOR was determined using the thickness of the specimen after con-ditioning. The MOR retention and IB retention are calcu-lated by the following relation:
MOR (or IB) retentionð%Þ
¼ Value after accelerated aging test Value before accelerated aging test100
The thickness change is calculated by the following relation:
Thickness change ð%Þ ¼ t1t0 t0
wheret0andt1are the air-dried thickness before and after the accelerated aging test, respectively.
Twelve specimens of PF board and MDI board measuring 300 9300 mm were set up on an exposure stand that (a) (b) (c) (d)
faced south at an angle of 90°to the ground. The cut edges of the specimens were coated with enamel paint as a waterproof agent prior to outdoor exposure. Two speci-mens were collected for testing at 1–5, 6 or 7 years to evaluate the board properties. The outdoor exposure was conducted at eight sites in Japan: Asahikawa, Morioka, Noshiro, Tsukuba, Shizuoka, Okayama, Maniwa, and Mi-yakonojo. Table1lists the latitude, longitude and climate conditions of these eight areas from February 2004 to March 2011. Details of the outdoor exposure can be found in the references [10,13–15].
The 3009300 mm specimens were also conditioned; in order to conduct the MOR tests, specimens measuring 280950 mm were taken from the 3009300 mm spec-imens. The moisture content of the specimens was approximately 10 % . After conditioning, MOR tests were then conducted. For subsequent TC and IB tests, specimens measuring 50950 mm were taken from the 280950 mm specimens. The trimming of MOR, TC, and IB specimens has been reported in previous studies [10, 13]. As the thickness of the 50950 mm specimens for TC test were not measured before outdoor exposure, the values were estimated from the mean thickness of the 3009300 mm specimens prior to outdoor exposure in
order to determine TC. The number of specimens of MOR, TC and IB were eight, thirteen and thirteen, respectively.
Results and discussion
Figure2a shows the relationships between soaking time and the TC of the PF board. The TC at 40 °C increased gradually with increasing soaking time, but was as low as 9 % at 336 h. The TC at 70 °C increased gradually with increasing soaking time, and was as low as 17 % at 168 h. The TC at 100°C was as high as approximately 20 %, even with a short soaking time of 1 h, and was thereafter almost constant with increasing soaking time.
Figure2b shows the relationships between soaking time and the TC of the MDI board. The TC at 40 °C increased at 12 h, but was as low as 6 % even at 336 h. The TCs at 70 and 100 °C increased with an increase in the soaking time, and the TC at 70°C at 168 h was the same as that at 100 °C at 72 h. In addition, the TC of the MDI board was much lower than that of the PF board. Though the PF and MDI boards were waterproof, their TCs increased after
Table 1 Latitude, longitude and climatic conditions for outdoor exposure sites from February 2004 to March 2011
Sites Groups North latitude (°) East longitude (°) Annual average temperature (°C) Annual precipitation (mm)
Asahikawa Northern Japan 43 142 7.3 992
Morioka Northern Japan 39 141 10.6 1,338
Noshiro Northern Japan 40 140 11.6 1,500
Tsukuba Northern Japan 36 140 14.4 1,371
Shizuoka Southern Japan 34 138 17.0 2,342
Maniwa Southern Japan 35 133 14.0 1,409
Okayama Southern Japan 34 133 16.7 1,069
Miyakonojo Southern Japan 31 131 16.9 2,515
Fig. 2 Relationships between
soaking them in water for a prolonged period of 336 h, even at 40°C.
Modulus of rupture
Figure3a shows the relationships between soaking time and the MOR retention of the PF board. The MOR reten-tion at 40°C decreased gradually with an increase in soaking time, but was as high as 70 % at 336 h. As at 40°C, the MOR retention at 70°C decreased to 56 % with increasing soaking time, and was lower than that at 40°C. The MOR retention at both 40 and 70°C decreased with increasing soaking time, while that at 100°C decreased to 59 %, even at 1 h, and subsequently was almost constant at approximately 60 %. It is obvious that a lower limit of approximately 60 % exists.
Figure3b shows the relationships between soaking time and the MOR retention of the MDI board. At 2 h, the MOR retention at 40°C was almost the same as that at 70°C, which was 90 %. Both decreased with increasing soaking time. The MOR retention at 40°C was 75 % at 336 h, while that at 70°C was 65 % at 168 h. On the other hand,
the MOR retention at 100°C was almost constant at approximately 65 % (lower limit) irrespective of soaking time.
The MOR retention of the MDI board is higher than that of the PF board, which results in a corresponding higher durability of the former. Additionally, the MOR retention of both the MDI and PF boards at 40°C did not decrease greatly with increasing soaking time, while that at 100°C decreased greatly for a short soaking time and subsequently was almost constant, irrespective of soaking time. On the other hand, the MOR retention at 70°C decreased with increasing soaking time, and finally reached almost the same retention at 100°C.
Figure4a shows the relationships between soaking time and the IB retention of the PF board. As in MOR, the IB retention at both 40 and 70 °C decreased with increasing soaking time. The IB retention at 70°C decreased more than that at 40°C, to 14 % at 168 h. On the other hand, IB at 100°C was almost constant at 10–20 % (lower limit),
Fig. 3 Relationships between
soaking time and MOR retention.MORmodulus of rupture.aPhenol–formaldehyde resin-bonded particleboard (PF board).bIsocyanate resin-bonded particleboard (MDI board)
Fig. 4 Relationships between
soaking time and IB retention. IBinternal bond strength.
irrespective of soaking time. The IB retention at 70°C at 168 h corresponded with that at 100°C in 24 h.
Figure4b shows the relationships between soaking time and IB retention of the MDI board. Although IB retention at 100°C for the PF board decreased to 19 % at 1 h, IB retention for the MDI board reached 73 % at 1 h, but decreased with an increase in the soaking time and dropped to 47 % (the lower limit) at 72 h.
In both the PF and MDI boards, IB retention was lower than MOR retention. In particular, the IB retention of the PF board at 100°C was very low. As IB is related to the bonding strength of the binder only , the bonding strength decreased because of water soaking, leading directly to a large decrease in IB. Although like IB, MOR is related to the bonding strength, it is also related to the particle shape [17–19], face-layer density , and many more factors. While the bonding strength decreased, these other factors were retained. Therefore, MOR did not decrease significantly and its value remained relatively unchanged as compared with the value of IB.
Reduction mechanism of board properties owing to water soaking
As discussed above, the MOR and the IB retention decreased when the TC increased. The MOR and IB are inversely related to the TC. Boards are manufactured through the high-density compression of particles, which generates significant local swelling stress within a board; this is the cause of spring-back when particles absorb water. Furthermore, particles swell when they absorb water. Spring-back and swollen particles are the causes of thickness swelling, which is controlled by the bonding strength of the binder at the bonding points among the particles (Fig.5) [9,10]. Water soaking causes a board to swell, thus collapsing the bonding points. Moreover, higher-temperature water soaking causes the board to swell to a greater extent , thus collapsing more bonding points. This is the reduction mechanism of board properties owing to water soaking. Thereby, when swelling stress is released completely and the boards have swollen to a
limited extent owing to water soaking, the remained bonding points do not collapse at all. The TCs of both the PF and MDI boards swollen to a limited extent are likely to be 20 and 9 %, respectively. With increased soaking time, the board does not swell beyond these TCs, and thus board properties do not markedly decrease. Therefore, lower limits for both MOR and IB exist. Therefore, water soaking as an accelerated aging test must be a short-time soaking to achieve the lower limits.
Reduction mechanism of board properties owing to outdoor exposure
The swollen thickness causes a reduction of board prop-erties owing to water soaking as discussed above, while it also causes a reduction in properties owing to outdoor exposure. Figure6a shows the relationships between TC and MOR retention of the PF board exposed outdoors for 1–7 years. The ‘‘Outdoor (North)’’ labels represent Asa-hikawa, Morioka, Noshiro and Tsukuba. The ‘‘Outdoor (South)’’ labels represent Shizuoka, Maniwa, Okayama, and Miyakonojo. This figure also includes the relationships between TC and MOR retention of the PF board soaked in water at various temperatures and times. The MOR reten-tion of both water soaking and outdoor exposure decreased with increasing TC. Moreover, the MOR retention of water soaking was higher than that of outdoor exposure. Figure6b shows the relationships between TC and IB retention of the PF board. The IB retention also decreased with increasing TC. Although the MOR retention of water soaking was higher than that of outdoor exposure (Fig.6a), the IB retention of water soaking was almost the same as that of outdoor exposure. The MOR decreases owing to the degradation of face layers , while the IB decreases owing to the degradation of the core layer [10,16]. Water soaking degrades both the face layers and the core layer together, while outdoor exposure degrades the face layers more severely than the core layer as the face layers are directly exposed to sunshine and rain. Thus, the MOR of outdoor exposure decreased more than that of water soaking.
Figure7a shows the relationships between the TC and MOR retention of the MDI board. As in the PF board, the MOR retention of water soaking was also higher than that of outdoor exposure, but the difference of the MDI board was less than that of the PF board. Figure7b shows the relationships between the TC and IB retention of the MDI board. The IB retention for both outdoor exposure and water soaking decreased with increasing TC. The IB retention of water soaking was slightly higher than that of outdoor exposure at TC of 7–10 %. Compared with the PF board, the TC of the MDI board exposed outdoors was much lower.
As for both the PF and MDI boards exposed outdoors, the TC of the north group was lower than that of the south group. Conversely, temperature and precipitation in the south group are higher, which presumably swells board thickness considerably . The swollen board forms many voids, presumably resulting in biodegradation . Therefore, both MOR retention and IB retention in the south group were lower.
Except for the IB of the PF board, as for the MOR of the PF board, the MOR and IB of the MDI board, there are differences between water soaking and outdoor exposure. In particular, the MOR retention of water soaking was higher than that of outdoor exposure. The boards soaked in water have poor mechanical properties solely because of the collapse of the bonding points, and the mechanism for the reduction of the properties is very simple. In contrast, the boards exposed outdoors have poor properties because of the collapse of the bonding points and biodegradation . These factors interact, resulting in a major reduction in the properties of the boards exposed outdoors than in the case of the boards
soaked in water. These differences between outdoor exposure and water soaking cause different reductions in the properties of both boards.
At 100°C, the MOR and IB retention of the PF board, and the MOR retention of the MDI board decreased to the lower limit for a soaking time of 1–2 h. At 70°C; a long soaking time is required to reach the lower limit. At 40°C, the lower limit could not be achieved, even for a long soaking time of 336 h. At 100 °C, the IB retention of the MDI board did not reach the lower limit for soaking time of 1–2 h, and 72 h was required to reach it. Thus a short-time soaking to reach the lower limit must be developed. In addition, because the reduction mechanism of the proper-ties of the boards soaked in water is different from that of the boards exposed outdoors, it is difficult to predict the durability of outdoor exposure on the basis of the resultant durability of water soaking.
Fig. 6 Effects of thickness
change on MOR retention (a) and IB retention (b) of PF board.MORmodulus of rupture,IBinternal bond strength,PF boardphenol– formaldehyde resin-bonded particleboard. Outdoor (North): Asahikawa, Morioka, Noshiro and Tsukuba; Outdoor (South): Shizuoka, Maniwa, Okayama and Miyakonojo
Fig. 7 Effects of thickness
Acknowledgments This study was supported by a Grant from LIXIL JS Foundation, a Grant-in-Aid for Scientific Research (21380108) from the Ministry of Education, Culture, Sports, Science and Technology of Japan, and an Emachu Research Fund. The authors are grateful for the grants received. The outdoor exposure test was conducted as part of a project organized by the Research Working Group on Wood-based Panels from the Japan Wood Research Society. The authors express their thanks to all participants in this project.
1. Kajita H, Mukudai J, Yano H (1991) Durability evaluation of particleboards by accelerated aging tests. Wood Sci Technol 25:239–249
2. Alexopoulos J (1992) Accelerated aging and outdoor weathering of aspen waferboard. Forest Prod J 42(2):15–22
3. McNatt JD, McDonald D (1993) Two accelerated-aging tests for wood-based panels. Forest Prod J 43(7/8):49–52
4. Japanese Industrial Standards (2003) JIS A 5908 JIS standard specification for particleboard, Japanese Standards Association, Tokyo
5. APA Standard (1994) PRP-108 Performance standards and pol-icies for structural-use panels. The Engineered Wood Products Association, Tacoma, WA
6. River BH (1994) Outdoor aging of wood-based panels and cor-relation with laboratory aging. Forest Prod J 44(11/12):55–65 7. Okkonen EA, River BH (1996) Outdoor aging of wood-based
panels and correlation with laboratory aging: part 2. Forest Prod J 46(3):68–74
8. Saotome H, Ohmi M, Tominaga H, Fukuda K, Kataoka Y, Kiguchi M, Hiramatsu Y, Miyatake A (2009) Improvement of dimensional stability and weatherability of composite board made from water-vapor-exploded wood elements by liquefied wood resin impregnation. J Wood Sci 55:190–196
9. Sekino N (2006) Evaluation and adhesion durability of wood-based panel (in Japanese). Wood Preservation 32:140–144
10. Korai H, Sekino N, Saotome H (2012) Effects of outdoor expo-sure angle on the deterioration of wood-based board properties. Forest Prod J 62:184–190
11. Horioka K, Horiike K, Noguchi M (1956) Researches for the improvement of wood (Rep. No. 3). Study on the mechanism of adhesion (part 1) (in Japanese). Bull Gov For Exp Station No 89:1–55
12. Korai H (2012) Improvement of acetylated fiberboard by ozoni-zation (in Japanese). J Adhesion Soc Jpn 48:30–35
13. Korai H, Adachi K, Saotome H (2013) Deterioration of wood-based boards subjected to outdoor exposure in Tsukuba. J Wood Sci 59:24–34
14. Korai H (2012) Durability of medium density fiberboard sub-jected to outdoor exposure (in Japanese). Mokuzai Gakkaishi 58:347–356
15. Sekino N, Korai H (2005) Second durability evaluation project of wood-based panel (in Japanese). J Timber Eng 18:110–117 16. Kawai S, Suda K, Sasaki H (1987) Production technology of
low-density particleboard IV. Effects of particle low-density and com-paction ratio on board properties (in Japanese). Mokuzai Gak-kaishi 33:385–392
17. Suda K, Kawai S, Sasaki H (1987) Production technology of low-density particleboard III. Effects of particle geometry on board properties. Mokuzai Gakkaishi 33:376–384
18. Canadido LS, Saito F, Suzuki S (1988) Effect of particle shape on the orthotropic properties of oriented strand board. Mokuzai Gakkaishi 34:21–27
19. Korai H, Ling N, Saito Y, Ebihara T (2010) Properties of oriented strand board manufactured from wood pallet waste (in Japanese). Mokuzai Gakkaishi 56:412–419
20. Wong ED, Zhang M, Wang Q, Kawai S (1998) Effects of mat moisture content and press closing speed on the formation of density profile and properties of particleboard. J Wood Sci 44:287–295